### Numerical study of molten metal melt pool behaviour during conduction-mode laser spot

### melting

Ebrahimi, Amin; Kleijn, C.R.; Richardson, I.M. DOI

10.1088/1361-6463/abca62

Publication date 2021

Document Version Final published version Published in

Journal of Physics D: Applied Physics

Citation (APA)

Ebrahimi, A., Kleijn, C. R., & Richardson, I. M. (2021). Numerical study of molten metal melt pool behaviour during conduction-mode laser spot melting. Journal of Physics D: Applied Physics, 54(10), [105304]. https://doi.org/10.1088/1361-6463/abca62

Important note

To cite this publication, please use the final published version (if applicable). Please check the document version above.

Copyright

Other than for strictly personal use, it is not permitted to download, forward or distribute the text or part of it, without the consent of the author(s) and/or copyright holder(s), unless the work is under an open content license such as Creative Commons. Takedown policy

Please contact us and provide details if you believe this document breaches copyrights. We will remove access to the work immediately and investigate your claim.

**J. Phys. D: Appl. Phys. 54 (2021) 105304 (19pp)** https://doi.org/10.1088/1361-6463/abca62

**Numerical study of molten metal melt**

**pool behaviour during conduction-mode**

**laser spot melting**

**Amin Ebrahimi**

1###

**, Chris R Kleijn**

2###

**and Ian M Richardson**

1###

1_{Department of Materials Science and Engineering, Delft University of Technology, Mekelweg 2, Delft}
2628 CD, The Netherlands

2_{Department of Chemical Engineering, Delft University of Technology, van der Maasweg 9, Delft 2629}
HZ, The Netherlands

E-mail:a.ebrahimi@tudelft.nl

Received 11 August 2020, revised 5 November 2020 Accepted for publication 13 November 2020 Published 22 December 2020

**Abstract**

Molten metal melt pools are characterised by highly non-linear responses, which are very sensitive to imposed boundary conditions. Temporal and spatial variations in the energy flux distribution are often neglected in numerical simulations of melt pool behaviour. Additionally, thermo-physical properties of materials are commonly changed to achieve agreement between predicted melt-pool shape and experimental post-solidification macrograph. Focusing on laser spot melting in conduction mode, we investigated the influence of dynamically adjusted energy flux distribution and changing thermo-physical material properties on melt pool oscillatory behaviour using both deformable and non-deformable assumptions for the gas-metal interface. Our results demonstrate that adjusting the absorbed energy flux affects the oscillatory fluid flow behaviour in the melt pool and consequently the predicted melt-pool shape and size. We also show that changing the thermo-physical material properties artificially or using a

non-deformable surface assumption lead to significant differences in melt pool oscillatory behaviour compared to the cases in which these assumptions are not made.

Keywords: laser material processing, melt pool behaviour, thermocapillary flow, flow instabilities, free surface oscillation

(Some figures may appear in colour only in the online journal)

**1. Introduction**

Laser melting is being utilised for material processing such as
additive manufacturing, joining, cutting and surface
*modifica-tion. The results of experimentation performed by Ayoola et al*
[1] revealed that the energy flux distribution over the melt-pool
surface can affect melting, convection and energy transport

Original Content from this work may be used under the terms of theCreative Commons Attribution 4.0 licence. Any further distribution of this work must maintain attribution to the author(s) and the title of the work, journal citation and DOI.

in liquid melt pools and the subsequent re-solidification
dur-ing laser meltdur-ing processes. The imposed energy flux heats
and melts the material and generates temperature gradients
over the melt-pool surface. The resulting surface tension
gradi-ents and therefore Marangoni force is often the dominant
force driving fluid flow, as can be understood virtually from
*the numerical investigation conducted by Oreper et al [*2] and
*experimental observations reported by Mills et al [*3].
*Experi-mental investigations of Heiple et al[*4] showed that the
pres-ence of surfactants in molten materials can alter Marangoni
convection in the melt pool, and thus the melt-pool shape.
*Moreover, Paul et al [*5] reported that the smoothness of the
melt pool surface decreases when surfactants are present in
the melt pool. However, according to the literature survey

*conducted by Cook et al [*6], the influence of surfactants on
variations of surface tension and its temperature gradient is
often neglected in numerical simulations of welding and
addit-ive manufacturing. DebRoy and David [7] stated that fluid
flow in melt pools can lead to deformation and oscillation of
the liquid free surface and can affect the stability of the
pro-cess and the structure and properties of the solid materials
*after re-solidification. Aucott et al [*8] confirmed that transport
phenomena during fusion welding and additive manufacturing
processes are characterised by highly non-linear responses that
are very sensitive to material composition and imposed heat
flux boundary conditions. Numerical models capable of
pre-dicting the melt pool behaviour with a sufficient level of
accur-acy are thus required to gain an insight into the physics of fluid
flow and the nature of flow instabilities that are not accessible
experimentally.

To avoid excessive simulation complexity and execution
time in numerical simulations, the melt pool in such
sim-ulations is often decoupled from the heat source, the latter
being incorporated as a boundary condition at the melt-pool
surface. These boundary conditions should be imposed with
a sufficient level of accuracy, as it is known from the work
*of Zacharia et al [*9] that modelling the interfacial
phenom-ena is critical to predicting the melt pool behaviour.
Numer-ical studies on melt pool behaviour reported in the
literat-ure use both deformable and non-deformable surface
assump-tions for the gas-metal interface. Comparing the melt-pool
shapes predicted using both deformable and non-deformable
surface assumptions, Ha and Kim [10] concluded that
free-surface oscillations can enhance convection in the melt pool
*and influence the melt-pool shape. Shah et al [*11] reported
that the difference between melt-pool shapes obtained from
numerical simulations with deformable and non-deformable
surface assumptions depends on the laser power.
Three-dimensionality of the molten metal flow in melt pools, as
*observed experimentally by Zhao et al [*12] and numerically by
*Kidess et al [*13], is often neglected in numerical simulations.
Moreover, when accounting for surface deformations, the
volume-of-fluid (VOF) method developed by Hirt and
Nich-ols [14], based on a Eulerian formulation, is the most common
method for modelling the melt pool behaviour. In this diffuse
boundary method, the interfacial forces and the energy fluxes
applied on the melt-pool surface are treated as volumetric
source terms in the surface region, instead of imposing them as
boundary conditions. In this approach, however, the fact that
surface deformations lead to temporal and spatial variations
of the free surface boundary conditions, as remarked by Meng

*et al [*15*] and Wu et al [*16], is often neglected. The results

*reported by Choo et al [*17] suggest that variations in
power-density distribution and changes in free-surface profile can
affect molten metal flow in melt pools and its stability. Further
investigations are essential to improve the understanding of the
complex transport phenomena that happen during laser spot
melting.

The aim of the present work is to analyse the effects of a dynamically adjusting energy flux distribution over the deforming liquid surface on the nature of fluid flow instabilities in partially-penetrated liquid melt pools. We will

particularly focus on flow instabilities in low-Prandtl number liquid metal pools during conduction-mode laser spot melting; our results should however be relevant for a much wider range of materials processing technologies. Three-dimensional cal-culations are carried out to numerically predict the melt pool behaviour and thermocapillary-driven flow instabilities using various heat source implementation methods. Our study provides a quantitative representation and an understanding of the influence of heat flux boundary conditions on the trans-port phenomena and flow instabilities in the molten metal melt pool. Additionally, we discuss the influence of artificially enhanced transport coefficients on the melt-pool oscillatory behaviour.

**2. Model description**
*2.1. Physical model*

Laser spot melting of a metallic S705 alloy, as shown
schematically in figure 1 and as experimentally studied by
*Pitscheneder et al [*18], was numerically simulated as a
rep-resentative example in the present work. A defocused
*laser-beam with a radius of r*b*= 1.4 mm heats the bulk *

*mater-ial from its top surface for 4 s. The laser-beam power Q is*
set to 3850 W with a top-hat intensity distribution. The
*aver-aged laser absorptivity of the material surface η is assumed*
to remain constant at 13% [18]. The absorbed laser power
leads to an increase in temperature and subsequent
melt-ing of the base material. The base material is a rectangular
*cuboid shape with a base size (L× L) of 24 × 24mm*2 and
*a height (H*m) of 10 mm, initially at an ambient

*temperat-ure of T*i*= 300 K. A layer of air with a thickness of H*a=

2 mm is considered above the base material to monitor the gas-metal interface evolution. Except for the surface tension, the material properties are assumed to be constant and tem-perature independent and are presented in table1. Although temperature-dependent properties can be employed in the present model to enhance the model accuracy, employing temperature-independent properties facilitates comparison of the results of the present work with previous results published in the literature [10,19,20], where temperature-independent material properties are employed. Moreover, further studies are required to enhance the accuracy of calculation and meas-urement of temperature-dependent material properties, partic-ularly for the liquid phase above the melting temperature. The effects of employing temperature-dependent material proper-ties on the thermal and fluid flow fields and melt-pool shape are discussed in detail in section4.3. A change in surface-tension due to the non-uniform temperature distribution over the gas– liquid interface induces thermocapillary stresses that drive the melt flow. This fluid motion from low to high surface-tension regions changes the temperature distribution in the melt pool [21] and can lead to surface deformations that change the melt-pool shape and properties of the material after solidification [22]. The sulphur contained in the alloy can alter the surface tension of the molten material and its variations with temper-ature [23].

**Figure 1.** Schematic of conduction-mode laser spot melting.

**Table 1.** Thermophysical properties of the Fe-S alloy and air used
in the present study. Values are taken from [20].

Property Fe-S alloy Air Unit

*Density ρ* 8100 1.225 kg m*−*3

*Specific heat capacity c*p 670 1006 J kg*−*1K*−*1
*Thermal conductivity k* 22.9 0.024 W m*−*1K
*Viscosity µ* 6*× 10−*3 1.8*× 10−*05 kg m*−*1s*−*1
*Latent heat of fusion L*f 250800 – J kg*−*1

*Liquidus temperature T*l 1620 – K

*Solidus temperature T*s 1610 – K

*2.2. Mathematical models*

A three-dimensional multiphase model based on the
finite-volume method was utilised to predict the melt pool dynamic
behaviour and the associated transport phenomena. The
present model is developed for conduction-mode laser
melt-ing. Further considerations will be required to develop the
model for keyhole mode welding, including the complex
laser-matter interactions, changes in surface chemistry and
con-sequent surface tension variations for non- or partially shielded
welding conditions. Both the molten metal and air were treated
as Newtonian and incompressible fluids. Thermal buoyancy
forces, which in laser spot melting are generally negligible
compared to thermocapillary forces [24], were neglected both
in the liquid metal and in the air. During conduction-mode
laser-melting, the heat-source energy density is too low to
cause significant vaporisation of the liquid metal [25], and the
surface deformations are too small to cause multiple
reflec-tions of the laser rays at the liquid surface [26]. Furthermore,
our preliminary results indicate that the maximum
temperat-ure of the melt pool is predominantly below 2700 K,
signi-ficantly less than the boiling temperature of stainless steels,
which is typically*O(3100)K. Hence, multiple reflections and*

vaporisation were ignored. With this, the unsteady
conserva-tion equaconserva-tions of mass, momentum and energy were defined
as follows:
*∇ ·**ρ⃗V*
*= 0,* (1)
*∂*
*∂t*
*ρ⃗V*
+*∇ ·*
*ρ⃗V⃗V*
=*−∇p + ∇ ·*
*µ∇⃗V*
*+ ⃗S*d*+ ⃗F*s*,*
(2)
*∂*
*∂t(ρh) +∇ ·*
*ρ⃗Vh*
=*∇ ·*
*k*
*c*p
*∇h*
*−* *∂*
*∂t(ρ∆H)*
*− ∇ ·**ρ⃗V∆H*
*+ S*T*,* (3)

*where ρ is density, t time, ⃗V velocity vector, p pressure, µ*
*dynamic viscosity, h sensible heat, k thermal conductivity, c*p

*specific heat capacity at constant pressure and ∆H latent heat.*
*The enthalpy of the material H was defined as the sum of the*
latent heat and the sensible heat [27], and is expressed as

*H = h + ∆H =*
*h*ref+
ˆ _{T}*T*ref
*c*p*dT*
*+ f*L*L*f*,* (4)

*where h*ref *is reference enthalpy, T*ref reference temperature,

*L*f*latent heat of fusion, and f*L local liquid volume-fraction.

Assuming the liquid volume-fraction in the metal to be a func-tion of temperature only, a linear funcfunc-tion [27] was used to calculate the liquid volume-fraction as follows:

*f*L=

*T− T*s

*T*l*− T*s

; *T*s*≤ T ≤ T*l*,* (5)

*where T*s *and T*l are the solidus and liquidus temperatures,

respectively.

To suppress fluid velocities in solid regions and to model fluid flow damping in the so-called “mushy zone”, where phase transformation occurs within a temperature range

*between T*s*and T*l*, a momentum sink term ⃗S*d[28] was

imple-mented into the momentum equation as

*⃗S*d*= C* (1*− f*L

)2

*f*3
L*+ ϵ*

*⃗ _{V,}*

_{(6)}

*where C is the mushy-zone constant and ε is a small number*
*to avoid division by zero as f*Lapproaches 0. The mushy-zone

*constant C was set to 10*7_{kg m}*−2*_{s}*−2*_{, which is large enough to}

dampen fluid velocities in solid regions according to the
*cri-terion defined by Ebrahimi et al [*29*], and ε was equal to 10−3*.
To capture the position of the gas–metal interface during
melting, the volume-of-fluid (VOF) method developed by Hirt
and Nichols [14] was utilised. This requires the solution of a
*transport equation for one additional scalar variable ϕ (i.e., the*
so-called volume-of-fluid fraction) that varies between 0 in the
gas phase and 1 in the metal phase:

*∂ϕ*
*∂t* +*∇ ·*
*ϕ⃗V*
*= 0.* (7)
Computational cells with 0*≤ ϕ ≤ 1 are in the gas-metal*
interface region. The effective thermophysical properties of
the fluid is then calculated using the mixture model as follows
[30]:

*ζ = ϕ ζ*_{metal}+ (1*− ϕ)ζ*gas*,* (8)

*where ζ corresponds to density ρ, viscosity µ, thermal *
*con-ductivity k and specific heat capacity c*p.

*Based on the method developed by Brackbill et al [*31],
surface tension and thermocapillary forces acting on the
gas-metal interface were applied as volumetric forces in these
interface cells and were introduced into the momentum
*equa-tion as a source term ⃗F*sas follows:

*⃗ _{F}*

s*=⃗f*s*∥∇ϕ∥ _{ρ}*

*2ρ*gas

*+ ρ*metal

*,* (9)

where subscripts indicate the phase. The term
*2ρ/(ρ*gas*+ ρ*metal) was utilised to abate the effect of the large

metal-to-gas density ratio by redistributing the
*volumet-ric surface-forces towards the metal phase (i.e., the heavier*
*phase).⃗f*sis the surface force per unit area and was defined as

follows:

*⃗f*s*= σκ⃗n +*

*dσ*

*dT*[*∇T −⃗n(⃗n · ∇T)],* (10)

where the first term on the right-hand side is the normal
com-ponent, which depends on the value of surface tension and
curvature of the melt-pool surface, and the second term is the
tangential component that is affected by the surface tension
gradient. In equation (10*), σ is surface tension, and κ the *
sur-face curvature is

*κ =−(∇ ·⃗n),* (11)

*and ⃗n the surface unit normal vector is*

*⃗n = _{∥∇ϕ∥}∇ϕ*

*.*(12)

**Table 2.** The values used to calculate the surface tension of molten
Fe–S alloy [23]

Property Value Unit

*σ*m*◦* 1.943 N m*−*1
*(∂σ/∂T)◦* *−4.3 × 10−*4 N m*−*1K*−*1
Γs 1.3*× 10−*5 mol m*−*2
*ψ* 3.18*× 10−*3 –
*a*s 150 –
*∆H◦* *−166.2 × 10*5 J mol*−*1

*2.2.1. Surface tension.* The temperature dependence of the
surface tension of a liquid solution with a low concentration of
surfactant can be approximated using a theoretical correlation
derived on the basis of the combination of Gibbs and Langmuir
adsorption isotherms as follows [32,33]:

*σ = σ◦− RTΓ*_{s}*ln(1 + Ka*s*),* (13)

*where σ is the surface tension of the solution, σ◦* the pure
*solvent surface tension, R the gas constant, Γ*sthe adsorption

*at saturation, K the adsorption coefficient, and a*sthe activity

*of the solute. From this, Sahoo et al [*23] derived a correlation
for binary molten metal–surfactant systems, including binary
Fe–S systems:
*σ = σ _{m}◦*+

*∂σ*

*∂T*

*◦*

*(T− Tm*)

*− RTΓ*sln

*1 + ψ a*sexp

*−∆H◦*

*RT*

*,*(14)

*where σ◦m*is the surface tension of pure molten-metal at the

*melting temperature Tm, ψ an entropy factor, ∆H◦*the

*stand-ard heat of adsorption, and (∂σ/∂T)◦*the temperature
coeffi-cient of the surface tension of the pure molten-metal. Values of
the properties used in equation (14) to calculate the
temperat-ure dependence of the surface tension of the molten Fe–S alloy
are presented in table2. Variations of the surface tension and
its temperature coefficient are shown in figure2for an Fe–S
alloy with 150 ppm sulphur content.

*2.2.2. Laser heat source.* The laser supplies a certain
*amount of energy (η Q) to the material. Its energy input was*
*modelled by adding a volumetric source term S*Tto the energy

equation (equation (3)) in cells at the gas–metal interface. The surface deformations affect the total energy input to the mater-ial [34]. This effect is generally not considered in numerical simulations of melt pool behaviour. To investigate the influ-ence of surface deformations, five different methods for the heat-source implementation were considered.

*2.2.2.1. Case 1, heat-source implementation without taking*
*the influence of surface deformations on total energy input*
*into consideration.* In this case, the heat source model is
defined as
*S*T=
(
*η Q*
*πr*2
b*∥∇ϕ∥*
*2 ρ c*p
*(ρ c*p)_{gas}*+(ρ c*p)_{metal}*,* *if r≤ r*b
*0,* otherwise (15)

**Figure 2.** Variations of surface tension (green solid-line) and its
temperature gradient (blue dashed-line) as a function of temperature
obtained from equation (14) for an Fe–S alloy containing 150 ppm
sulphur.

*where r is radius defined as*p*x*2* _{+ y}*2

_{. This method is the most}

common method in modelling melt-pool surface oscillations
without having a deep penetration (keyhole formation) (see
for instance, [25,26]). However, variations in the total energy
input caused by a change in melt-pool surface shape, through
changes in*∥∇ϕ∥, causing*˝

*∀* *S*T*dV to be different from ηQ,*

are an inherent consequence of using this method. Addition-ally, every segment of the melt-pool surface is exposed to the same amount of energy input regardless of the local surface orientation.

*2.2.2.2. Case 2, heat source adjustment.* To conserve the
*total energy input, an adjustment coefficient ξ was introduced*
to the heat source model as follows:

*S*T=
(
*ξ η Q*
*πr*2
b*∥∇ϕ∥*
*2 ρ c*p
*(ρ c*p)gas*+(ρ c*p)metal
*,* *if r≤ r*b
*0,* otherwise (16)
*where ξ was evaluated at the beginning of every time-step and*
was defined as

*ξ =* ˝*η Q*

*∀* *S*T*dV*

*,* (17)

where*∀ stands for the computational domain. Utilising this*
technique for welding simulations has already been reported in
the literature (see for instance, [15,16,34,35]). Variations in
energy absorption with deformations of the melt-pool surface
are, however, not taken into consideration in this method.

*2.2.2.3. Case 3, heat source redistribution.* In this case,
the energy flux was redistributed over the melt-pool surface
assuming the energy absorption is a function of the local
sur-face orientation. Accordingly, the local energy absorption is a
maximum where the surface is perpendicular to the laser ray

and is a minimum where the surface is aligned with the laser ray [36,37]. This represents a simplified absorptivity model based on the Fresnel’s equation [38] and is expressed math-ematically, assuming the laser rays being parallel and in the

*z-direction, as follows:*
*S*T=
(
*η Q*
*πr*2
b*∥∇ϕ∥*
*2 ρ c*p
*(ρ c*p)gas*+(ρ c*p)metal
*∇ϕ[z] _{∥∇ϕ∥}*

*. ifr ≤ r*b

*0.*otherwise (18) the total energy input is not necessarily conserved in this method.

*2.2.2.4. Case 4, heat source redistribution and adjustment.*

Utilising the same technique introduced in Case 2, the heat
source model in Case 3 was adjusted to guarantee that total
energy input is conserved. Hence, the heat source model was
defined as
*S*T=
(
*ξ η Q*
*πr*2
b*∥∇ϕ∥*
*2 ρ c*p
*(ρ c*p)gas*+(ρ c*p)metal
*∇ϕ[z] _{∥∇ϕ∥}*

*. ifr ≤ r*b

*0.*otherwise (19)

*2.2.2.5. Case 5, Flat non-deformable free surface.* In this
case, the surface was assumed to remain flat. Thermocapillary
shear stresses caused by a non-uniform temperature
distribu-tion on the gas-metal interface were applied as a boundary
con-dition, hence modelling the gas phase was not required.
Con-sequently, the total energy absorbed by the surface was fixed
in this method. The boundary conditions are described in
sec-tion2.2.3.

Table3presents a summary of the cases considered in the present work.

*2.2.3. Boundary conditions.* The bottom and lateral
sur-faces of the metal part were modelled to be no slip walls,
but in fact they remain solid during the simulation time. At
the boundaries of the gas layer above the metal part, a
*con-stant atmospheric pressure was applied (i.e., p = 101.325 kPa)*
allowing air to flow in and out of the domain. The outer
bound-aries of the computational domain were modelled as adiabatic
since heat losses through these boundaries are negligible
com-pared to the laser power [20].

For Case 5, in which no gas layer is modelled explicitly, a
thermocapillary shear-stress was applied as a boundary
condi-tion in the molten regions of the top surface. In the irradiated
region on the material top-surface, a constant uniform heat
flux was applied, while outside of this region the surface was
assumed to be adiabatic [18]. The thermal and thermocapillary
shear-stress boundary conditions were defined, respectively,
as
*k∂T*
*∂⃗n* =
(
*η Q*
*πr*2
b
*,* *if r≤ r*b
*0,* otherwise (20)

**Figure 3.** Comparison of the numerically predicted melt-pool shape after 5 s of heating with the corresponding experimentally measured
*post-solidification melt-pool shape reported by Pitscheneder et al [*18]. Laser power was set to 3850 W and the material contains 150 ppm
sulphur. Numerical predictions obtained from the present model assuming (a) non-deformable (Case 5) and (b) deformable gas-metal
interface (Case 4).
and
*− µ∂ ⃗V*t
*∂⃗n* =
*dσ*
*dT*
*∂T*
*∂⃗τ,* (21)

*where ⃗V*t*is the tangential velocity vector, and ⃗τ the tangential*

vector to the top surface.

**3. Numerical procedure**

The model was developed within the framework of the
pro-prietary computational fluid dynamics solver ANSYS
Flu-ent [39]. The laser heat source models and the
thermocapil-lary boundary conditions as well as the surface-tension model
were implemented through user-defined functions. After
per-forming a grid independence study (results are presented
in appendix A), a grid containing 8.6*× 10*5 non-uniform
hexahedral cells was utilised to discretise the computational
domain. Minimum cell spacing was 2*× 10−5*m close to the
gas-metal interface and 3*× 10−5* m in the melt pool
cent-ral region. Cell sizes gradually increase towards the domain
outer boundaries. The computational domain employed in the
numerical simulations is shown in appendixA. The diffusion
and convection terms in the governing equations were
discret-ised using the central-differencing scheme with second order
accuracy. For the pressure interpolation, the “pressure
stagger-ing option” (PRESTO) scheme [40] was used. Pressure and
velocity fields were coupled employing the “pressure-implicit
with splitting of operators” (PISO) scheme [41]. An explicit
compressive VOF formulation was utilised for the spatial
dis-cretisation of the gas-metal interface advection [42]. The
tran-sient advection terms were discretised using a first order
impli-cit scheme. To obtain a Courant number (Co =*∥⃗V∥∆t/∆x)*
less than 0.25, with velocity magnitudes up to *O(1)ms−1*,
the time-step size was set to 10*−5*s. Each simulation was
executed in parallel on 40 cores (Intel Xeon E5-2630 v4)
of a high-performance computing cluster. Scaled residuals of
the energy, momentum and continuity equations of less than

**Table 3.** Summary of the cases studied in the present work and the
features included in the model for each case.

Name Deformable free-surface Heat source adjustment Heat source redistribution Case 1 Yes No No

Case 2 Yes Yes No

Case 3 Yes No Yes

Case 4 Yes Yes Yes

Case 5 No No No

10*−10*, 10*−8* and 10*−7*respectively, were defined as
conver-gence criteria.

**4. Results and discussion**

*4.1. Model validation and solver verification*

To verify the reliability and accuracy of the present
numer-ical simulations, the melt-pool shapes obtained from the
present simulations, for the problem introduced in
sec-tion 2.1, are compared to experimental observations
*repor-ted by Pitscheneder et al [*18]. Figure3 shows a comparison
between the melt-pool shape obtained from the numerical
sim-ulation after 5 s of heating and the post-solidification
experi-mental observation, which indicates a reasonable agreement.
The maximum absolute deviations between the present
numer-ical predictions and experimental data for the melt-pool width
and depth is less than 5% and 2%, respectively. However,
it should be noted that the thermal conductivity and
viscos-ity of the liquid material were artificially increased in the
simulations by a factor *F = 7 with respect to their *
*repor-ted experimental values, as suggesrepor-ted by Pitscheneder et al*
[18]. This is known as employing an ‘enhancement factor’,
mainly to achieve agreement between numerical and
experi-mental results [19]. Independent studies conducted by Saldi

**Figure 4.** Comparison of the spot melt-pool shape obtained from the present numerical simulation with the corresponding experimentally
observed (the right side of the figure) and numerically predicted (the left side of the figure) post-solidification melt-pool shape reported by
*He et al [*49]. Laser power was set to 1967 W and the beam radius was 570 µm. Blue circles show the melt-pool shape predicted using the
present model. The 500 mm s*−*1reference vector is provided for scaling the velocity field shown in the melt pool.

such an enhancement factor, the fluid flow structure and the
melt-pool shape in simulations differ drastically from
exper-imental observations. The use of an enhancement factor is
often justified by the possible occurrence of turbulence and
its influence on heat and momentum transfer in the melt pool,
which is assumed to be uniform in the melt pool. However, the
*high-fidelity numerical simulations conducted by Kidess et al*
[13,20] on a melt pool with a flat non-deformable melt-pool
surface revealed that turbulent enhancement is strongly
*non-uniform in the melt pool, resulting in an ω-shaped melt pool*
that differs notably from the results of simulations assuming
uniform transport enhancement. We extended this study and
performed a high-fidelity simulation based on the large eddy
simulation (LES) turbulence model and took the effects of
sur-face deformations into consideration [44] and showed that for
the conduction-mode laser melting problem we considered,
the influence of surface oscillations on melt pool behaviour
is larger compared to the effects of turbulent flow in the melt
pool; nevertheless the results do not agree with experiments
without using some enhancement. These observations along
with previous studies [19,43,45] suggest that the published
weld pool models lack the inclusion of significant physics. The
neglect in simulations of relevant physics such as chemical
reactions and unsteady oxygen absorption by the melt-pool
surface, non-uniform unsteady surfactant distribution over the
melt-pool surface, re-solidification, free surface evolution and
three-dimensionality of the fluid flow field has been postulated
*as reasons why such an ad hoc and unphysical enhancement*
factor is needed to obtain agreement with experimental data
[46–48]. However, the inclusion of such factors will increase
the model complexity and computational costs. Further
invest-igations are essential to realising the problem with sufficient
details. In section4.4, the effects of the value used for the
enhancement factor*F on the thermal and fluid flow fields and*
melt-pool oscillatory behaviour are discussed in more detail.

*The experimental and numerical data reported by He et al*
[49], who investigated unsteady heat and fluid flow in the melt
pool during conduction-mode laser spot welding of stainless
steel (AISI304) plates, were considered to validate the
reli-ability of the present model. The melt pool shape obtained

from the present model assuming a non-deformable free
sur-face (Case 5) was compared with experimental and numerical
*data reported by He et al [*49] and the results are shown in
fig-ure4. In this problem, the laser power was set to 1967 W, the
beam radius was 570 µm and laser pulse duration was 3 ms.
The thermal conductivity and viscosity of the molten
mater-ial were artificmater-ially increased in the simulations by a factor

*F = 17 and F = 11, respectively, as suggested by He et al*

[49]. The maximum absolute deviations between the present numerical predictions and experimental data for the melt-pool width and depth is less than 8% and 2.5%, respectively. The results obtained from the present model are indeed in reason-able agreement with the reference data, indicating the validity of the present model in reproducing the results reported in lit-erature.

The reliability of the present model was also investigated by
comparing the numerically predicted melt-pool size and
sur-face deformations with experimental observations of
*Cunning-ham et al [*50]. The evolutions of the melt-pool shape and its
surface depression under stationary laser melting of a
Ti-6Al-4V plate under conduction mode were studied. In this problem,
the laser power is 156 W and has a Gaussian distribution and
the radius of the laser spot is 7*× 10−5*m. The thermophysical
*properties of Ti-6Al-4V suggested by Sharma et al [*51] were
employed for calculations. Since the melt pool surface
temper-ature reaches the boiling point, the effects of recoil pressure

*p*r*and evaporation heat loss q*ewere included in the model.

The recoil pressure [52] and evaporation heat loss [53] were determined respectively as follows:

*p*r*= 0.54· P*0exp
*L*v*M (T− T*v)
*R T T*v
*,* (22)
*q*e=*−0.82√L*v*M*
*2πM R TP*0exp
*L*v*M (T− T*v)
*R T T*v
*,* (23)

*where P*0*is the ambient pressure, L*vthe latent heat of

**Figure 5.** Comparison of (a) the melt-pool surface depression and (b) the melt pool aspect ratio (depth to width ratio) obtained from the
*present numerical simulation with the corresponding experimental observations of Cunningham et al [*50]. Laser power was set to 156 W
and the beam radius was 70 µm. Snapshots of the melt pool and its deformed surface are shown in the right subfigure for three different time
instances.

*the temperature and T*v= 3315 K the evaporation

temperat-ure. The results obtained from the present numerical
simula-tions using the heat source model introduced for Case 4 are
*compared with those reported by Cunningham et al [*50] in
figure5, which show a reasonable agreement. The maximum
absolute deviations between the present numerical predictions
and experimental data for the melt-pool aspect ratio is less than
12%.

Particular attention was also paid to the effect of spurious
currents on numerical predictions of molten metal flow in melt
pools with free surface deformations. Spurious currents are
an unavoidable numerical artefact generating unphysical
para-sitic velocity fields that do not vanish with grid refinement
when using the continuum surface force technique for
model-ling surface tension effects in the VOF method. This problem
*has been thoroughly investigated by Mukherjee et al [*54] and
the results of their study show that the Reynolds number based
on the time-averaged maximum spurious velocity is*O(10).*
The results of the present simulations show that the flow
Reyn-olds number is*O(10*3_{) that is at least two orders of magnitude}

larger than that induced by spurious currents. Furthermore, to suppress fluid velocities in the solid regions a momentum sink term is defined based on the enthalpy porosity technique that further weakens the spurious currents in solid regions. There-fore, the influence of spurious currents on numerical predic-tions is considered to be negligible in the present study.

*4.2. The influence of heat source adjustment*

When accounting for surface deformations, the volume-of-fluid (VOF) method developed by Hirt and Nichols [14], based on a Eulerian formulation, is the most common method for modelling the melt pool behaviour. In this diffuse boundary method, the interfacial forces and the energy fluxes applied on the melt-pool surface are treated as volumetric source terms in the surface region, instead of imposing them as boundary conditions. In this approach, however, the fact that surface

deformations lead to temporal and spatial variations of the free
*surface boundary conditions, as remarked by Meng et al [*15]
*and Wu et al [*16], is often neglected. The results reported by
*Choo et al [*17] suggest that variations in power-density
dis-tribution and changes in free-surface profile can affect molten
metal flow in melt pools and its stability. In this section, the
influence of applying each of the five different approaches to
model the laser heat source (described as Cases 1–5 in
sec-tion 2.2.2) on the melt pool behaviour is discussed. In these
simulations, no enhancement factor, as introduced in the
*pre-vious section, was employed since it is ad hoc and has little*
justification in physical reality.

The energy flux distribution over the melt-pool surface
determines the spatial temperature distribution over the
melt-pool surface and its temporal variations. Due to the
tem-poral changes in the melt-pool surface shape, the total energy
*absorbed by the material in Case 1 varies between 491.4 W*
*and 538.1 W, with a median value of 515.7 W, which differs*
*from the total energy supplied by the laser η Q = 500.5 W.*
This issue is resolved by utilising a dynamic adjustment
coef-ficient in Case 2, while the relative energy flux distribution
remains unchanged. However, the results reported by Courtois

*et al [*55*] and Bergström et al [*56] showed that the energy

flux distribution varies with surface deformation during a laser
melting process. When surface deformations are too small to
cause multiple reflections, redistributing the energy flux over
the free surface results in a better input energy conservation as
obtained in Case 3. The total energy absorbed by the material
*in Case 3 ranges between 482.6 W and 532.3 W, with a median*
*value of 503.8 W. By further introducing an adjustment *
coef-ficient (equation (17)), the absorbed energy can be made to
*exactly match the supplied laser power ηQ. Finally, for the*
*most simple approach without any surface deformations (i.e.,*
Case 5), the total absorbed energy exactly matches the
sup-plied laser power and remains unchanged in time.

The variations of temperature distribution over the melt-pool surface over time determine the thermocapillary driven

**Figure 6.** Contours of temperature and the velocity vectors on the melt pool free surface at two different time instances for Cases 1, 4 and 5.
*Coordinates are non-dimensionalised using the laser-beam radius r*bas the characteristic length scale.

**Figure 7.** Variations of the averaged angular momentum over the
melt-pool surface over a time period of 4 s for (a) Case 1, (b) Case
2, (c) Case 3, (d) Case 4 and (e) Case 5. Unfiltered data: grey lines,
*Moving average of the data over 0.05 s: dashed blue lines.L > 0*
indicates a clockwise rotation.

flow pattern and melt-pool shape, as shown in figure6. An unsteady, asymmetric, outwardly directed fluid flow eman-ating from the pool centre is found for all 5 cases. Flow

accelerates towards the pool rim, where it meets inwardly
dir-ected fluid flow from the rim, due to the change of sign of
*(∂σ/∂T) at a certain pool temperature (see figure*2). Close to
the region where these two flows meet, velocity magnitudes
are high due to the large thermocapillary stresses generated
by the steep temperature gradients, in contrast to the low flow
velocities in the central region of the pool surface. Interactions
between these two opposing flows, and their interactions with
the fusion boundary, cause the fluid flow inside the melt pool
to be asymmetric and unstable [20], leading to a distorted
melt-pool shape.

Melt-pool surface temperatures are roughly 7–16% higher
when surface deformations are taken into consideration (Cases
1–4), compared to flat surface simulations (Case 5).
Temper-ature gradients over the melt-pool surface are also on average
larger in Cases 1–4 (with a deformable surface) and
particu-larly in Cases 2–4 (with heat source adjustment and/or
redis-tribution), compared to Case 5 (with a non-deformable
sur-face). Consequently, local fluid velocities caused by
thermo-capillary stresses are almost 25% higher for Cases 1–4,
*com-pared to those of Case 5, and are of the order of 0.6 ms−1*, in
reasonable agreement with experimental measurements
*per-formed by Aucott et al [*8] and estimated values from the
scal-ing analyses also reported by Oreper and Szekely [2], Rivas
and Ostrach [57] and Chakraborty and Chakraborty [58].

Free surface deformations have a destabilising effect on the melt pool due to the augmentation of temperature gradi-ents over the melt-pool surface, leading to higher thermo-capillary stresses [59]. Additionally, the stagnation region,

**Figure 8.** Contours of melt pool free surface deformation at three different time instances for (a) Case 1, (b) Case 2, (c) Case 3, and (d)
*Case 4. Coordinates are non-dimensionalised using the laser-beam radius r*bas the characteristic length scale. Positive and negative values
*of z indicate surface depression and elevation, respectively.*

*where the sign of (∂σ/∂T) and thus thermocapillary flow *
dir-ection change, is sensitive to small spatial disturbances and
further enhances melt pool instabilities. Furthermore,
vari-ations in magnitude and direction of velocities can cause
rota-tional and pulsating fluid motions, leading to cross-cellular
flow patterns with a stochastic behaviour in the melt pool
[12,60].

All such flow instabilities reinforce unsteady energy trans-port from the melt pool to the surrounding solid material, resulting in continuous melting and re-solidification of the

material close to the solid-liquid boundary. This complex interplay leads to the melt-pool surface width for Case 5 to be 23% smaller than that for Case 1, and 10% smaller than for Cases 2–4. The higher amount of heat absorbed by the deformed free-surface in Case 1, and the enhanced convective heat transfer in Cases 1–4, are the main causes for the observed pool size differences.

To investigate the rotational fluid motion, the
spatially-averaged angular momentum over the melt-pool surface (*L )*
*about the z-axis (i.e. the axis of rotation) with respect to the*

**Figure 9.** *Contours of melt-pool depth at t = 3.98 s and 4.00 s for Cases 1, 4 and 5. Coordinates are non-dimensionalised using the*
*laser-beam radius r*bas the characteristic length scale. The orange circular line shows the melt pool boundary at its top surface.

**Figure 10.** *(a) Temperature signals recorded from the monitoring point p*4*located at (x∗, y∗) = (0, 0) on the melt-pool surface and (b) the*
corresponding frequency spectra. Temperature signals in the period of 1–4 s are employed for FFT analysis.

origin*O(0,0,0) is calculated as follows:*

*L (t) =* 1
*A*
¨
free surface
ˆ*z·*
*⃗r× ⃗V*
*dA,* (24)
*where ˆz is a unit vector in the z-direction, ⃗r the position *
*vec-tor, ⃗V velocity vector and A the area of gas-metal interface.*
Figure7shows the temporal variations of angular momentum
over the melt-pool surface as a function of time. Positive
val-ues of the angular momentum in figure7 show a clockwise
*flow rotation, and vice versa. Kidess et al [*20] applied a similar

approach to investigate rotational fluid motion over a flat
non-deformable melt-pool surface. Continuous fluctuations in the
sign of angular momentum indicate an oscillatory rotational
fluid motion in the pool that is indeed self-excited. In Cases
1–4, flow pulsations start to take place after roughly 1 s and
continue thereafter. This is not however valid for Case 5,
*where flow pulsations start to occur already after about 0.1 s,*
*and a clockwise rotation is established after 1.8 s, which lasts*
for roughly two seconds. These instabilities in the flow field
are attributed to a large extent to the interactions between
the two opposing flows meeting at the melt-pool surface

**Figure 11.** Temperature signals recorded from three monitoring
points at the melt pool free surface placed at a radius of 1 mm and
*along different azimuthal directions (p*1*(x∗, y∗) = (5/7, 0),*

*p*2*(x∗, y∗) = (5/7, 5/7) and p*3*(x∗, y∗) = (0, 5/7)). (a) Case 1, (b)*
Case 4, and (c) Case 5. Signals are smoothed using a moving
*averaging window of 0.01 s.*

[13,20], and to a lesser extent the effects of hydrothermal waves [61,62].

Free surface deformations evolve rapidly because of the
thermocapillary stresses acting on the melt-pool surface and
are shown in figure8 at three different time instances. Free
surface deformations are smaller and less intermittent in Case
1 compared with Cases 2–4. This is due to the smaller
ther-mocapillary stresses and the wider stagnation region, which
makes the surface flow field less sensitive to spatial
*disturb-ances. Additionally, the Capillary number (Ca = µ∥⃗V∥/σ),*
which represents the ratio between viscous and
surface-tension forces and which is*O(10−3*) for all the cases
stud-ied in the present work, appears to be larger in Cases 2–4

(Ca*≈ 2.5 × 10−3*) compared with Case 1 (Ca*≈ 1.5 × 10−3*),

particularly in the central region of the melt-pool surface. Redistributing the energy flux based on the free surface profile (Cases 3 and 4) disturbs the temperature field locally and thus the velocity distribution over the melt-pool surface.

Fluid flow may influence the energy transport and associ-ated phase change significantly during laser melting [7], which can be assessed through the P´eclet number that is the ratio between advective and diffusive heat transport, defined as fol-lows:

Pe =*D∥⃗V∥ρc*p

*k* *,* (25)

where*D is a characteristic length scale, here chosen to be r*b.

The value of the P´eclet number is much larger than one (Pe =

*O(10*2_{)), which indicates a large contribution of advection to}

the total energy transport, compared with diffusion.

The predicted melt-pool depth is shown in figure 9 at two different time instances. When surface deformations are

taken into account (Cases 1–4), the predicted melt-pool shape is shallow, with its maximum depth located in the central region and its largest width at the surface. When the surface is assumed to be non-deformable (Case 5), the depth profile of the melt-pool resembles a doughnut-shaped, with its max-imum width located below the gas-metal interface. The pre-dicted fusion boundaries of all the cases studied in the present work are asymmetric and unstable. Flow instabilities in the melt pool increase when surface deformations are taken into account, which enhance convection in the pool resulting in a smooth melt-pool depth profile. Variations in the melt-pool shape for Case 5 are less conspicuous compared to those for Cases 1–4 because of the smaller fluctuations in the fluid flow field.

To understand the three-dimensional oscillatory flow
beha-viour, three monitoring points were selected over the
*melt-pool surface in different non-azimuthal directions p*1*(x∗, y∗*) =

*(5/7, 0), p*2*(x∗, y∗) = (5/7, 5/7) and p*3*(x∗, y∗) = (0, 5/7) in*

*addition to a point p*4*(x∗, y∗) = (0, 0) on the melt-pool *

*sur-face, in which x** * _{and y}**

_{are non-dimensionalized with the}

*laser beam radius r*b. Temperature signals, recorded from the

*monitoring point p*4, and the corresponding ‘fast Fourier

trans-form’ (FFT) [63] frequency spectra are shown in figure10. In the presence of surface deformations (Cases 1–4), self-excited temperature fluctuations, initiated by numerical noise, grow and reach a quasi-steady state after about 1 s. Without surface deformations (Case 5), the amplitudes of temperat-ure fluctuations remain very small. In Case 1, where surface deformations are taken into account, the temperature fluctu-ations with large amplitudes have a fundamental frequency of

*f*0*≈ 22 Hz, with harmonics at f*1*≈ 2f*0 *and f*2*≈ 3f*0.

Irregu-lar patterns appear in the spectrum of temperature fluctuations for Case 2–4, showing a highly unsteady behaviour that res-ults from the enhancement of thermocapillary stresses and the variations in energy flux distribution.

*Temperature signals recorded from monitoring points p*1*, p*2

*and p*3in the time interval of 2–3 s are shown in figure11. The

data for Case 1 indicate that the thermal and fluid flow fields
are dominated by a pulsating behaviour. This is also valid
*for Case 4 up to roughly 2.5 s; however, after 2.5 s *
modula-tion of temperature fluctuamodula-tions takes place, which is probably
due to changes in temperature gradients, melt pool size and
the complex interactions between vortices generated inside the
melt pool. Similar behaviour was observed for Cases 2 and 3
(not shown here). The amplitudes of temperature fluctuations
appear to be smaller for Case 5 compared to the other cases
and show an irregular behaviour, revealing complex unsteady
flow in the melt pool.

*4.3. The effects of employing temperature-dependent*
*material properties*

In this section, the effects of employing temperature-dependent properties on numerical predictions of thermal and flow fields as well as the melt-pool shape are investig-ated using two different heat source models (Cases 1 and 4). Temperature-dependent properties for the metallic alloy

**Table 4.** Temperature-dependent thermophysical properties of the Fe–S alloy used in the present study. Values are estimated by analogy
with the values for iron-based alloys [64].

Property Fe-S alloy Unit

*Density ρ* 8100 kg m*−*3

*Specific heat capacity c*p 627 (solid phase) J kg*−*1K*−*1

723.14 (liquid phase)

*Thermal conductivity k* 8.8521+0.0114*·T (solid phase)* W m*−*1K*−*1

4.5102+0.0107*·T (liquid phase)*

*Viscosity µ* *0.0659− 7 × 10−*5*· T + 3 × 10−*8*·*

*T*2*− 3 × 10−*12*· T*3

kg m*−*1s*−*1

*Latent heat of fusion L*f 250 800 J kg*−*1

*Thermal expansion coefficient β* 2*× 10−*6 K*−*1

*Liquidus temperature T*l 1620 K

*Solidus temperature T*s 1610 K

**Figure 12.** Contours of temperature and the velocity vectors on the melt pool free surface after 5 s of heating predicted using the heat source
models Cases 1 and 4 with temperature-dependent (table4) and temperature-independent (table1) material properties. Coordinates are
*non-dimensionalised using the laser-beam radius r*bas the characteristic length scale.

**Figure 13.** Contours of melt-pool depth at 5 s for Cases 1 and 4 predicted using temperature-dependent and temperature-independent
*material properties. Coordinates are non-dimensionalised using the laser-beam radius r*bas the characteristic length scale. The orange
circular line shows the melt pool boundary at its top surface.

considered in the present study (S705) are given in table4,
where the values are estimated by analogy with the values
for iron-based alloys [64]. Temperature distribution over the
melt-pool surface and free-surface flow after 5 s of
heat-ing are shown in figure 12 for both temperature-dependent
and temperature-independent thermophysical properties.
Melt-pool surface temperatures predicted using
temperature-independent properties are about 1–6% lower than those
predicted using temperature-dependent properties. This is
mainly attributed to the changes in the thermal diffusivity
*(α = k/ (ρc*p)) of the molten material. The thermal

*conduct-ivity of the molten material changes from 21.8 W m−1*K*−1*
*at T = 1620 K to 33.4 W m−1*K*−1at T = 2700 K. Hence, the*
average thermal diffusivity of the molten material obtained
from a temperature-dependent model is about 10% lower than
that estimated using temperature-independent properties. The

fluid velocities are roughly 15–32% lower when
temperature-independent properties are employed, compared to those
predicted using temperature-dependent properties, which is
due to the decrease in the viscosity of the molten
mater-ial at elevated temperatures. With an increase in
temperat-ure, the thermal conductivity of the molten metal increases
and the viscosity of the molten metal decreases, resulting in
a reduction of momentum diffusivity and enhancement of
thermal diffusivity and thus reduction of the Prandtl
*num-ber (Pr = c*p*µ/k). Although the heat source models affect*

the thermal and flow fields in the melt pool, it is found that the numerical predictions are less sensitive to the heat source models when temperature-dependent properties are employed for the cases studied in the present work. How-ever, it should be noted that for the cases where surface deformations are larger, the effects of heat source adjustment

**Figure 14.** The influence of employing temperature-dependent material properties on temperature signals received from the melt pool and
*the corresponding frequency spectra. (a) Temperature signals recorded from the monitoring point p*4*located at (x∗, y∗) = (0, 0) on the*
melt-pool surface and (b) the corresponding frequency spectra. Temperature signals in the period of 1–5 s are employed for FFT analysis.

**Figure 15.** *(a) Temperature signals recorded from the monitoring point p*4*(x∗, y∗) = (0, 0) on the melt-pool surface and (b) the*

corresponding frequency spectra for different values of the enhancement factor*F. Temperature signals in the period of 1–4s are employed*
for FFT analysis.

on numerical predictions become critical, as discussed in section4.2.

Changes in the material properties with temperature affect thermal and flow fields in the melt pool, resulting in changes in the predicted melt-pool shape, as shown in figure13. When temperature-dependent properties are employed, the melt-pool depth is significantly (about 36–74%) larger than that predicted using temperature-independent properties.

Temperature signals recorded from the monitoring point

*p*4and the corresponding frequency spectra are shown in

fig-ure 14. Temperature signals received from the monitoring
*point p*4are almost in the same range and vary between 2320 K

and 2820 K. Employing temperature-dependent properties affects the frequency spectra of fluctuations, however the amp-litude of fluctuations remains almost unaffected. The results presented in figure14indicate that adjusting the heat source dynamically during simulations can result in a decrease in the amplitude of temperature fluctuations, however its effect on the frequency spectrum is insignificant.

*4.4. The effects of the enhancement factor*

In section 4.1 it was mentioned that, in many simulation
studies in literature, the thermal conductivity and viscosity
of the liquid metal were artificially increased by a so-called
enhancement factor *F, in order to obtain better agreement*
between experimental and simulated post-solidification
*melt-pool shapes. Numerical studies carried out by De et al [*65–67]
showed that the values reported for the enhancement factor
in the literature depend greatly on operating conditions and
ranges from 2 to 100 (see for instance, [68–71]), however
val-ues between 2 and 10 are most often employed. The effects of
the enhancement factor*F on thermal and fluid flow fields in*
molten metal melt pools as well as the melt-pool shape can be
found in [19,43,45], thus are not repeated here. Focusing on
Case 4 in which free surface deformations are accounted for,
the influence of*F on the oscillatory flow behaviour is *
*invest-igated. Temperatures recorded from the monitoring point p*4

**Figure 16.** Temperature variations predicted at the melt pool centre
using different grid sizes. The grid with minimum cell spacing of
20 µm was employed for the calculations reported in the paper.

**Figure 17.** The computational grid employed for the present
calculations reported in the paper. Regions highlighted in blue show
the gas layer above the base material.

Temperatures and the amplitudes of fluctuations reduce with
increasing *F. The contribution of diffusion in total energy*
transport increases with*F, which results in a reduction of *
tem-perature gradients and therefore thermocapillary stresses
gen-erated over the melt-pool surface. The reduced
thermocapil-lary stresses in addition to the enhanced viscosity of the
mol-ten metal lead to a reduction of fluid velocities that decrease
convection in the melt pool further, which significantly affects
the fluid flow structure. Increasing*F to 2.5 results in *
relat-ively deeper melt pool with a corresponding reduction of the

fundamental frequency of fluctuations. Using higher values of

*F, the melt-pool shape approaches a spherical-cap shape and*

the frequency spectrum becomes rather uniform with small amplitude fluctuations.

**5. Conclusions**

Molten metal melt pool behaviour during a laser spot melting process was studied to investigate the influence of dynamic-ally adjusted energy flux distribution on thermal and fluid flow fields using both deformable and non-deformable gas–metal interfaces.

For the material and laser power studied in the present work, self-excited flow instabilities arise rapidly and fluid flow inside the melt pool is inherently three-dimensional and unstable. Flow instabilities in the melt pool have a significant influence on solidification and melting by altering the thermal and fluid flow fields. Free surface deformations, even small compared to the melt pool size, can significantly influence the fluid flow pattern in the melt pool. When in the numerical simulations the gas-metal interface is assumed to remain flat and non-deformable, lower temperatures with smaller fluctu-ations were found in comparison to those of the cases with a deformable interface, which results in a different melt-pool shape. Taking the surface deformations into account leads to erratic flow patterns with relatively large fluctuations, which are caused by the intensified interactions between vor-tices generated in the melt pool resulting from the augmen-ted thermocapillary stresses. When surface deformations are taken into account, various tested methods for adjusting the absorbed energy flux resulted in smaller melt-pool sizes com-pared to those without an adjustment. However, the melt pool behaves quite similarly for various adjustment methods stud-ied in the present work. This should be noted that the util-isation of temperature-dependent properties can enhance the accuracy of numerical predictions in simulations of molten metal flow in melting pools; however, the results presented in the present work show the importance of employing a physically-realistic heat-source model that is also applicable if temperature-dependent properties were employed.

Although the enhancement factors are widely used to achieve agreement between numerically predicted melt-pool sizes and solidification rates with experiments, they do not rep-resent the physics of complex transport phenomena governing laser spot melting. The use of an enhancement factor can sig-nificantly affect the numerical predictions of melt pool oscil-latory behaviour.

**Author contributions**

Conceptualisation, A E, C R K and I M R; methodology, A E; software, A E; validation, A E; formal analysis, A E; investig-ation, A E; resources, A E, C R K, and I M R; data curinvestig-ation, A E; writing—original draft preparation, A E; writing—review

**Table A1.** The influence of computational cell size on predicted
melt pool size.

Minimum cell spacing

Total number of cells

Melt pool

width Melt pool depth

60 µm 5.5*× 10*5 4.89 mm 1.09 mm

20 µm 8.6*× 10*5 4.88 mm 0.96 mm

10 µm 2.1*× 10*6 4.88 mm 0.95 mm

and editing, A E, C R K, and I M R; visualisation, A E; super-vision, C R K and I M R; project administration, A E and I M R; and funding acquisition, I M R.

**Conflict of interest**

The authors declare no conflict of interest.

**Acknowledgments**

This research was carried out under project number F31.7.13504 in the framework of the Partnership Program of the Materials innovation institute M2i (www.m2i.nl) and the Foundation for Fundamental Research on Matter (FOM) (www.fom.nl), which is part of the Netherlands Organisation for Scientific Research (www.nwo.nl). The authors would like to thank the industrial partner in this project “Allseas Engineering B V” for the financial support.

**Appendix A. Grid independence test**

Case 1 was considered for grid independence test. Three
dif-ferent grids with minimum cell spacings of 60, 20 and 10 µm
were studied. The influence of computational cell size on
pre-dicted melt pool depth and width are reported in tableA1,
which indicate the predictions are reasonably independent of
the grid size. The variations of temperature at the centre of the
*melt pool surface (i.e., T(0, 0, z*surface)) were also investigated

for different grid sizes and the results are shown in figure16. The grid with minimum cell size of 20 µm was employed for the present calculations reported in the paper, and is shown in figure17.

**ORCID iDs**

Amin Ebrahimihttps://orcid.org/0000-0002-4912-2549

Chris R Kleijnhttps://orcid.org/0000-0001-6821-0969

Ian M Richardsonhttps://orcid.org/0000-0002-3651-3233

**References**

[1] Ayoola W, Suder W and Williams S 2017 Parameters
controlling weld bead profile in conduction laser welding
*J. Mater. Process. Technol.***249 522–30**

[2] Oreper G M and Szekely J 1984 Heat- and fluid-flow
*phenomena in weld pools J. Fluid Mech.***147 53**
[3] Mills K C, Keene B J, Brooks R F and Shirali A 1998

*Marangoni effects in welding Phil. Trans. R. Soc. A*
**356 911–25**

[4] Heiple C R and Roper J R 1982 Mechanism for minor element
* effect on GTA fusion zone geometry Weld J. 61 97s–102s*
[5] Paul A and DebRoy T 1988 Free surface flow and heat transfer

*in conduction mode laser welding Metall. Trans. B*
**19 851–8**

[6] Cook P S and Murphy A B 2020 Simulation of melt pool
behaviour during additive manufacturing: Underlying
*physics and progress Additive Manuf.***31 100909**
[7] DebRoy T and David S A 1995 Physical processes in fusion

*welding Rev. Mod. Phys.***67 85–112**

*[8] Aucott L et al 2018 Revealing internal flow behaviour in arc*
*welding and additive manufacturing of metals Nat.*
*Commun.***9 5414**

[9] Zacharia T, David S A, Vitek J M and Debroy T 1990
*Modeling of interfacial phenomena in welding Metall.*
*Trans. B***21 600–3**

[10] Ha E-J and Kim W-S 2005 A study of low-power density laser
*welding process with evolution of free surface Int. J. Heat*
*Fluid Flow***26 613–21**

[11] Shah A, Kumar A and Ramkumar J 2018 Analysis of transient
thermo-fluidic behavior of melt pool during spot laser
*welding of 304 stainless-steel J. Mater. Process. Technol.*
**256 109–20**

[12] Zhao C, Kwakernaak C, Pan Y, Richardson I, Saldi Z,
Kenjeres S and Kleijn C 2010 The effect of oxygen on
*transitional marangoni flow in laser spot welding Acta*
*Mater.***58 6345–57**

[13] Kidess A, Kenjereš S, Righolt B W and Kleijn C R 2016
Marangoni driven turbulence in high energy surface melting
*processes Int. J. Thermal Sci.***104 412–22**

[14] Hirt C and Nichols B 1981 Volume of fluid (VOF) method for
*the dynamics of free boundaries J. Comput. Phys.*

**39 201–25**

[15] Meng X, Qin G and Zou Z 2016 Investigation of humping
defect in high speed gas tungsten arc welding by numerical
*modelling Mater. Des.***94 69–78**

[16] Wu D, Nguyen A V, Tashiro S, Hua X and Tanaka M 2019
Elucidation of the weld pool convection and keyhole
formation mechanism in the keyhole plasma arc welding
*Int. J. Heat Mass Transfer***131 920–31**

[17] Choo R T C, Szekely J and Westhoff R C 1990 Modeling of
high-current arcs with emphasis on free surface phenomena
**in the weld pool Weld J. 69 346–61**

[18] Pitscheneder W, DebRoy T, Mundra K and Ebner R 1996 Role
of sulfur and processing variables on the temporal evolution
of weld pool geometry during multikilowatt laser beam
**welding of steels Weld J. 75 71–80**

[19] Saldi Z, Kidess A, Kenjereš S, Zhao C, Richardson I and
Kleijn C 2013 Effect of enhanced heat and mass transport
and flow reversal during cool down on weld pool shapes in
*laser spot welding of steel Int. J. Heat Mass Transfer*
**66 879–88**

[20] Kidess A, Kenjereš S and Kleijn C R 2016 The influence of
surfactants on thermocapillary flow instabilities in low
*prandtl melting pools Phys. Fluids***28 062106**

[21] Heiple C R, Roper J R, Stagner R T and Aden R J 1983
Surface active element effects on the shape of GTA, laser
**and electron beam welds Weld J. 62 72s–77s**

[22] Mills K C and Keene B J 1990 Factors affecting variable weld
*penetration Int. Mater. Rev.***35 185–216**

[23] Sahoo P, Debroy T and McNallan M J 1988 Surface tension of binary metal—surface active solute systems under

*conditions relevant to welding metallurgy Metall. Trans. B*
**19 483–91**

[24] Zacharia T, Eraslan A H, Aidun D K and David S A 1989
Three-dimensional transient model for arc welding process
*Metall. Trans. B***20 645–59**

[25] Cho J, Farson D F, Hollis K J and Milewski J O 2015

Numerical analysis of weld pool oscillation in laser welding
*J. Mech. Sci. Technol.***29 1715–22**

[26] Kim Y-D and Kim W-S 2008 A numerical analysis of heat and
fluid flow with a deformable curved free surface in a laser
*melting process Int. J. Heat Fluid Flow***29 1481–93**
[27] Voller V R and Swaminathan C R 1991 General source-based

*method for solidification phase change Numer. Heat*
*Transfer B***19 175–89**

[28] Voller V and Prakash C 1987 A fixed grid numerical
modelling methodology for convection-diffusion mushy
*region phase-change problems Int. J. Heat Mass Transfer*
**30 1709–19**

[29] Ebrahimi A, Kleijn C R and Richardson I M 2019 Sensitivity
of numerical predictions to the permeability coefficient in
simulations of melting and solidification using the
*enthalpy-porosity method Energies***12 4360**

[30] Sun Y and Beckermann C 2004 Diffuse interface modeling of
two-phase flows based on averaging: mass and momentum
*equations Phys. D***198 281–308**

[31] Brackbill J, Kothe D and Zemach C A 1992 continuum
*method for modeling surface tension J. Comput. Phys.*
**100 335–54**

[32] Belton G R 1976 Langmuir adsorption, the Gibbs adsorption
isotherm and interracial kinetics in liquid metal systems
*Metall. Trans. B***7 35–42**

*[33] March N H and Tosi M P 1991 Atomic Dynamics in Liquids*
(New York: Dover)

[34] Gao X, Wu C, Goecke S and Kügler H 2017 Numerical
simulation of temperature field, fluid flow and weld bead
formation in oscillating single mode laser-GMA hybrid
*welding J. Mater. Process. Technol.***242 147–59**
[35] Ebrahimi A, Kleijn C R and Richardson I M 2021 A

simulation-based approach to characterise melt-pool
*oscillations during gas tungsten arc welding Int. J. Heat*
*Mass Transfer***164 120535**

[36] Arrizubieta J I, Lamikiz A, Klocke F, Martínez S, Arntz K and
Ukar E 2017 Evaluation of the relevance of melt pool
*dynamics in laser material deposition process modeling Int.*
*J. Heat Mass Transfer***115 80–91**

[37] Amara E H and Fabbro R 2010 Modeling of humps formation
*during deep-penetration laser welding App. Phys. A*
**101 111–16**

[38] Indhu R, Vivek V, Sarathkumar L, Bharatish A and
Soundarapandian S 2018 Overview of laser absorptivity
*measurement techniques for material processing Lasers*
*Manuf. Mater. Process.***5 458–81**

[39] ANSYS®*Fluent Release 18.1*

*[40] Patankar S V 1980 Numerical Heat Transfer and Fluid Flow,*
1st edn (London: Taylor & Francis Inc)

[41] Issa R 1986 Solution of the implicitly discretised fluid flow
*equations by operator-splitting J. Comput. Phys.***62**

40–65

[42] Ubbink O 1997 Numerical prediction of two fluid systems
*with sharp interfaces Doctoral Thesis Imperial College*
London University of London London, United Kingdom
(http://hdl.handle.net/10044/1/8604)

[43] Ehlen G, Ludwig A and Sahm P R 2003 Simulation of
time-dependent pool shape during laser spot welding:
*Transient effects Metall. Mater. Trans. A***34 2947–61**
[44] Ebrahimi A, Kleijn C R and Richardson I M 2019 The

influence of surface deformation on thermocapillary flow
instabilities in low Prandtl melting pools with surfactants
*Proc. 5th World Congress on Mechanical, Chemical and*
*Material Engineering (Avestia Publishing)*

(https://doi.org/10.11159/htff19.201)

[45] Mundra K, DebRoy T, Zacharia T and David S A 1992 Role of
*thermophysical properties in weld pool modeling Weld J.*
**71 313–20**

[46] Do-Quang M, Amberg G and Pettersson C-O 2008
Modeling of the adsorption kinetics and the convection
*of surfactants in a weld pool J. Heat Transfer*

**130 092102**

[47] Winkle C, Amberg G, Inoue H, Koseki T and Fuji M 2000
Effect of surfactant redistribution on weld pool shape
*during gas tungsten arc welding Sci. Technol. Weld. Join.*
**5 8–20**

[48] Tsai M C and Kou S 1989 Marangoni convection in weld
*pools with a free surface Int. J. Numer. Methods Fluids*
**9 1503–16**

[49] He X, Fuerschbach P W and DebRoy T 2003 Heat transfer and
*fluid flow during laser spot welding of 304 stainless steel J.*
*Phys. D: Appl. Phys.***36 1388–98**

[50] Cunningham R, Zhao C, Parab N, Kantzos C, Pauza J, Fezzaa
K, Sun T and Rollett A D 2019 Keyhole threshold and
morphology in laser melting revealed by ultrahigh-speed
*x-ray imaging Science***363 849–52**

[51] Sharma S, Mandal V, Ramakrishna S and Ramkumar J 2018
Numerical simulation of melt hydrodynamics induced hole
blockage in quasi-CW fiber laser micro-drilling of TiAl6V4
*J. Mater. Process. Technol.***262 131–48**

[52] Lee J Y, Ko S H, Farson D F and Yoo C D 2002 Mechanism of
keyhole formation and stability in stationary laser welding
*J. Phys. D: Appl. Phys.***35 1570–6**

*[53] von Allmen M and Blatter A 1995 Laser-Beam Interactions*
*With Materials (Berlin: Springer)*

[54] Mukherjee S, Zarghami A, Haringa C, van As K, Kenjereš S
and den Akker H E V 2018 Simulating liquid droplets: A
quantitative assessment of lattice Boltzmann and volume of
*fluid methods Int. J. Heat Fluid Flow***70 59–78**

[55] Courtois M, Carin M, Masson P L, Gaied S and Balabane M
2016 Guidelines in the experimental validation of a 3D heat
*and fluid flow model of keyhole laser welding J. Phys. D:*
*Appl. Phys.***49 155503**

[56] Bergström D, Powell J and Kaplan A F H 2007 A ray-tracing
analysis of the absorption of light by smooth and rough
*metal surfaces J. Appl. Phys.***101 113504**

[57] Rivas D and Ostrach S 1992 Scaling of low-Prandtl-number
*thermocapillary flows Int. J. Heat Mass Transfer*
**35 1469–79**

[58] Chakraborty N and Chakraborty S 2007 Thermal transport
regimes and generalized regime diagram for high energy
*surface melting processes Metall. Mater. Trans. B*
**38 143–7**

[59] Davis S H and Homsy G M 1980 Energy stability theory for
*free-surface problems: buoyancy-thermocapillary layers J.*
*Fluid Mech.***98 527**

[60] Czerner S 2005 Schmelzbaddynamik beim
*Laserstrahl-Wärmeleitungsschweiβen von Eisenwerkstoffen PhD*
*Thesis Leibniz Universität Hannover (*http://nbn-resolving.
de/urn: nbn:de:gbv:089-4942690490)

[61] Kuhlmann H C and Schoisswohl U 2010 Flow instabilities in
*thermocapillary-buoyant liquid pools J. Fluid Mech.*
**644 509**

*[62] Davis S H 1987 Thermocapillary instabilities Annu. Rev. Fluid*
*Mech.***19 403–35**

[63] Temperton C 1985 Implementation of a self-sorting in-place
*prime factor FFT algorithm J. Comput. Phys.*

**58 283–99**

*[64] Mills K C 2002 Recommended Values of Thermophysical*
*Properties for Selected Commercial Alloys (Cambridge:*
Woodhead)

[65] De A and DebRoy T 2006 Improving reliability of heat
and fluid flow calculation during conduction
mode laser spot welding by multivariable
*optimisation Sci. Technol. Weld. Join.*
**11 143–53**

[66] De A and DebRoy T 2005 Reliable calculations of heat and
fluid flow during conduction mode laser welding
*through optimization of uncertain parameters Weld J.*
**84 101–12**

[67] De A and DebRoy T 2004 A smart model to estimate effective
*thermal conductivity and viscosity in the weld pool J. Appl.*
*Phys.***95 5230–40**

[68] Zhang W, Roy G G, Elmer J W and DebRoy T 2003 Modeling
of heat transfer and fluid flow during gas tungsten arc spot
*welding of low carbon steel J. Appl. Phys.***93 3022–33**
[69] Choo R T C and Szekely J 1994 Possible role of turbulence in

**GTA weld pool behavior Weld J. 73 25–31**

[70] Mundra K and DebRoy T 1993 Toward understanding alloying
element vaporization during laser beam welding of stainless
**steel Weld J. 72 1–9**

[71] Choo R T C, Szekely J and Westhoff R C 1992 On the
calculation of the free surface temperature of
gas-tungsten-arc weld pools from first principles: part I. modeling the
*welding arc Metall. Mater. Trans. B***23 357–69**